- Email: [email protected]

S0010-4655(14)00203-3 http://dx.doi.org/10.1016/j.cpc.2014.05.029 COMPHY 5356

To appear in:

Computer Physics Communications

Received date: 25 October 2013 Revised date: 13 May 2014 Accepted date: 25 May 2014 Please cite this article as: M. Robinson, N.A. Marks, NanoCap: A framework for generating capped carbon nanotubes and fullerenes, Computer Physics Communications (2014), http://dx.doi.org/10.1016/j.cpc.2014.05.029 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

NanoCap: A Framework for Generating Capped Carbon Nanotubes and Fullerenes M. Robinson∗ Nanochemistry Research Institute, Department of Chemistry, Curtin University, Perth, WA 6845, Australia

N.A. Marks Discipline of Physics & Astronomy, Curtin University, Perth, WA 6845, Australia

Abstract NanoCap provides both libraries and a standalone application for the construction of capped nanotubes of arbitrarily chirality and fullerenes of any radius. Structures are generated by constructing a set of optimal dual graph topologies which are subsequently optimised using a carbon interatomic potential. Combining this approach with a GUI featuring 3D rendering capabilities allows for the rapid inspection of physically sensible structures which can be used as input for molecular simulation. Keywords: nanotubes, fullerenes, modelling PACS: 61.48.De, 61.48.-c, 07.05.Tp,33.15.-e PROGRAM SUMMARY

Manuscript Title: NanoCap - A Generator for Capped Carbon Nanotubes and Fullerenes Authors: Marc Robinson Program Title: NanoCap Journal Reference: Catalogue identifier: Licensing provisions: Creative Commons AttributionNonCommercial 2.5 (CC BY-NC 2.5) Programming language: Python, C Computer: Any system with Python (with NumPy and SciPy) and a C compiler. Operating system: Linux, OS-X, Windows RAM: up to 4 GB Keywords: Molecular Modelling, Atomistic Simulation, Fullerene, Nanotube Classification: 16.1 Molecular Physics and Physical Chemistry - Structure and Properties External routines/libraries: NumPy[1], SciPy [2], EDIP [3], (GUI version: Qt+PySide [4], VTK [5]) Nature of problem: The ability to readily produce arbitrary sized, low-energy fullerene and capped nanotube structures for molecular simulation. Solution method: Structures are generated using the dual lattice represen∗ Corresponding author. Address: Curtin University, GPO Box U1987, Perth, Western Australia. Tel.: +61 8 9266 3780. Email address: [email protected] (M. Robinson∗ )

Preprint submitted to Elsevier

tation, which are subsequently optimised using physical carbon interatomic potentials. Running time: Scales dependent on the number of carbon atoms in the structure. For the C196 molecule 10 structures can be found in around 30 seconds on a single CPU.

References [1] T. E. Oliphant. Comp. Sci. Eng. 9(3):1020 (2007). http://www.numpy.org [2] E. Jones, T. E. Oliphant, P. Peterson et al. SciPy: Open Source Scientific Tools for Python. http://www.scipy.org [3] N. A. Marks. Phys. Rev. B 63(3):035401 (2000). [4] Digia. Qt - Cross-platform application and UI framework. http://www.qt-project.org/ [5] W. Schroeder. K. Martin, B. Lorensen. The Visualisation Toolkit (1993-2008) http://www.vtk.org/

1. Introduction An immediate problem facing computational scientists who wish to model the physical and chemical properties of fullerenes or non-periodic capped nanotubes is the generation of sensible initial atomic coordinates. On one hand, highly symmetric topologies are readily available, such as icosahedral fullerenes which can be modified to terminate nanotubes of certain chiralities. A common example is the capping of May 5, 2014

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

its dual lattice equivalent. This idea is illustrated in Fig. 1 which shows the connection between the carbon network and its face dual lattice triangulation. Notably, the duality demonstrated is reversible, the ability to generate the triangular mesh allows extraction of the 3-fold coordinate carbon network and vice-versa. Therefore, construction of the dual lattice implicitly produces a carbon lattice and herein lies the advantage of this approach; generating the dual lattice is simpler and faster.

the (5,5) or (9,0) nanotubes with a section of the C60 fullerene. The construction of capped nanotubes using this approach is severely limited as the choice of nanotube chirality is constrained to known fullerene structures. Alternatively, complete enumeration of fullerene and cap topologies is possible when treating the carbon network as a 3-regular graph [1, 2]. However, as the number of carbon atoms increases, the number of possible topological arrangements grows exponentially. As a result, additional optimisation and analysis is required to produce a set of physically sensible structures. An application that enabled a computer modeller to quickly and directly generate a set of energetically favourable fullerene or capped nanotube structures would undoubtedly be a useful tool. At the time of writing, there are two applications available which explicitly enable the construction of fullerenes and capped nanotubes. Nanotube Modeler [3] is capable of constructing both capped nanotubes and fullerenes, however options are limited particularly with regards to nanotube caps where only five simple chiralities [(9,0), (5,5), (6,6), (10,0) and (10,10)] are available. A larger number of fullerene structures are available but it is not possible to produce fullerene of arbitrarily diameter. The capping of nanotubes using sections of fullerenes can also be carried out using generic visualisation and data manipulation tools such as Virtual NanoLab part of the Atomistix ToolKit [4]. FullGen [1, 2] part of the CaGe software package also enables the generation of fullerenes and capped nanotubes but adopts a purely mathematical approach. This application is useful for the enumeration of structures and identifies the associated symmetry groups. Unlike the application described in this paper, FullGen does not attempt to produce physically sensible, low energy structures nor does it produce structures containing heptagons which may be important for studies of defects. The fundamental function of the NanoCap application is the construction of physically sensible fullerene and capped nanotube topologies for use in atomistic computer simulations. To achieve this goal, the algorithms outlined are highly generalised such that fullerenes of any radius and capped nanotubes of arbitrary chirality can be constructed. Such a level of generalisation is possible due to the underlying concept behind the approach: the carbon lattice itself is not constructed but instead construction involves

Dual lattice point Carbon atom

(a)

(b)

(c)

Figure 1: The connection between the carbon lattice (solid black spheres) and the face dual representation (larger grey spheres). (a) A graphene layer. (b) The (5,5) nanotube, which is constructed by rolling the graphene layer shown in (a). (c) The C60 fullerene and its dual lattice the truncated icosahedron, which is typically used to cap the (5,5) nanotube. Bonds are shown between neighbouring carbon atoms.

The reason for the relative ease in which the dual lattice is produced becomes apparent when considering the lattice as close packed arrangement of spheres. This arrangement can be constructed by maximising the distance between the centre point of each sphere. A way of achieving this is to assign a repulsive potential energy function to each point and minimise the net total energy. This approach is analogous to a well studied problem, The Thomson Problem [5, 6, 7, 8, 9, 10, 11, 12, 13], which concerns the minimum energy arrangement of point charges on the surface of a sphere. The applicability of the proposed algorithm was recently demonstrated through the construction and examination of caps for nanotubes of various chiralities [14]. The reader is directed to this study for an overview of literature specific to the construction of nanotube caps. Using Density Functional Tight Binding (DFTB) to accurately model the carbon system, this work validated the ability of the approach to 2

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

produce low energy cap topologies. This conclusion emphasised the value of the approach and provided the motivation for the development of NanoCap.

START

2. Algorithm Flow Chart

False

An overview of the algorithms present in NanoCap is shown in Fig. 2. The core procedures (represented by rectangles with double-struck vertical edges) vary in complexity but fundamentally involve the creation, manipulation or analysis of point sets. Each routine is described in the proceeding sections following the order illustrated in Fig. 2.

If Capped Nanotube

True

Nanotube Dual Lattice Initialisation Fullerene Dual Lattice Initialisation Cap Dual Lattice Initialisation

n=0, nu=0 Dual Lattice

3. Fullerene Dual Lattice Initialisation If n == Nmax

The initial set of fullerene dual lattice points are produced by randomly distributing points on the sphere. This is achieved by drawing two random numbers, z0 =[−1,1] and t0 =[0,2π], which are then used to construct the cartesian coordinates: √ xi = √1 − z0 cos(t0 ) yi = 1 − z0 sin(t0 ) (1) z i = z0

STOP

False n ++

Escape Minimum

Dual Lattice Optimisation

False

If New Structure True

During the dual lattice optimisation process, a single point is fixed at the pole to constrain the rotational degrees of freedom of the system during the search for alternate structures. An additional point may also be held on the equator to further reduce the generation of symmetry equivalent structures.

Triangulation

Carbon Lattice Topology

If Full Optimisation

4. Nanotube Dual Lattice Initialisation Algorithms for the generation of uncapped nanotubes are well documented [15, 16] and typically concern the construction nanotubes that are periodic along the tube axis. However, producing finite capped nanotubes removes the requirement of such periodicity and a simpler approach to nanotube generation can be adopted. Fundamentally, the construction of a nanotube involves the transformation from a single 2D sheet of graphene. To correspond to the eventual construction of the nanotube, the 2D axis are labelled x and z, where z represents the nanotube axis. As illustrated in Fig. 3, this sheet is traditionally defined using two lattice vectors a1 and a2 : √ √ c a1 = 3a (2) 2 ( 3, 1) √ √ c a2 = 3a (3) 2 ( 3, −1)

True

False

True

Carbon Lattice Optimisation

Carbon Lattice

Output & Analysis

nu ++

False

If nu == Nu True

STOP

Figure 2: Flow diagram for the construction of a carbon fullerene or capped nanotube. Each core process (represented by rectangles with double-struck vertical edges) is explained in the text. In the above diagram, Nu indicates the number of unique structures to be found. Nmax limits the minima searching procedure.

3

dR =

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

d 3d

work of Saito et al. Using this vector the position of (1) The boundary along R with respect to periodic wrapthe i-th A atom is defined simply as iR. All other ping is defined as: The magnitude of C gives the circumference of the points in the basis, including the B atom are then R = pa1 + qa2 (7) |T| nanotube and as such the position of any point proRm = o↵set (12) from this position along a proportion of C and sin(✓Ch 6 R ) where the coefficients p and q are derived as in the jected onto C is proportional to the angle around the work of Saito et al. Using the 2 atom basis of the T.that All atom positions are generated from i=0 to NH , which is used to wrap positions of A atoms leave The radius of unit the cell. nanotube rt distance along graphene lattice, thenanotube. position of the i-th cylindrical A atom is the nanotube The additional where NH is the number of hexagons in the graphene defined simply as iR.isThe B atom is thenby o↵set also defined C:from T to the centre of a hexagon is given by: sheet: this position along a proportion of Ch and T. All

if nfined. − m is not a multiple of 3d,of The position if n − m is a multiple of 3d.

each atom is given by a sym-

metry vector R,

atom positions are generated from i=0 to Nhex , where Nhex is the number of hexagons in the graphene sheet. rt Application of the symmetry vector R to all sites un-

h

i

⇡ |C| ✓Ch B = ac · sin 6 (5) (13) (9) NH = 2(n2 + m2 + nm)/dR 2⇡ hex = 2 B with the cartesian axis. 2 which is used to determine the scaling factor to When the application of the symmetry vector genreduce the nanotube to a cylinder unit radius. The ofconstruction of each point P in the 2D erates coordinates outside of the nanotube cell posi( =1/rt ). tions are wrapped using the appropriate projection T graphene lattice The angle C subtends with the axis of the graphene is carried out row by row along C. onto C and T. 0° sheet is labelled the chiral angle ✓ as shown in C These rows are indicated in Fig. 3 andthecontain As introduced previously, algorithmn+m for cap Fig 3. Two special cases of nanotube are constructed construction isrow basedare uponproduced solving the Thomson points. The points in each iterawhen ✓C equals 0 [C=(n, 0)] and 30 [C=(n, n)]. problem using the dual lattice presentation of the These achiral nanotubes are known aswith the zigzag tively, theandpoint at iteration i given graphene network. Therefore, the by: two atom basis is armchair respectively and have additional mirror modified to incorporate a dual lattice point, which C plane symmetry when compared to chiral [C=(n, m)] is positioned in the centre of a hexagon as shown in nanotubes. PiFig=4.nUpon + mi a2 of the nanotube, this (7) i a1 construction gives Perpendicular to C is the vector T that defines the 30° Ntube =N dual lattice points. In addition to the genH z D axial length of the nanotube unit cell. Although not eration of carbon atomsto and(n, dualm). lattice points, a1 with from (0,0) The three innecessary for cap construction, T is(n defined that i , msuch i ) ranging other basis points are constructed. These points repthe nanotube is periodic along the nanotube axis. As crementation of m or n is dependent on: resent intersections of local carbon bonds (which are i i x such, T extends to the atom corresponding to the a2 also located at intersections of neighbouring dual latfirst atom at the origin of 2D unit cell and is given in tice points) and are denoted I1 to I3 . Each of these terms of a1 and a2 : ni ++ if mi /(2n + mi ) >a potential m/(2nC+ m) pointsi represents 2 axis of rotational (8) symmetry once the 3D nanotube is constructed. This m ++ if m /(2n + m ) ≤ m/(2n + m) i i T = t1 a1 + t2 a2 i (6) i Figure 3: Definition of the 2D lattice points P used for nanis useful in later routines involving transformations otube construction. At each point, the basis shown in Fig. 4 As T defines the smallest periodic unit, the coeffiof the final cap structure. The full basis is shown Each new except row foris translated in the using z direction cients t1the andchiral t2 have no common in Fig 4 and by translation R produces allby the is constructed. Points are constructed in rows along √ divisors unity andExample are given by: points required for nanotubeadded construction. 3a . Rows of points are continually until the vector as indicated by the graduated colour scale.

=

c

current length of 4the nanotube surpasses a user defined length. The minimum length is governed by the force cutoff described in Section 6.1 which is proportional to the density of dual lattice points in the cap. Performing the capping procedure with the shortest nanotube possible significantly reduces computational expensive, particularly in triangulation and rendering routines. At each point in the 2D nanotube lattice basis points are required as shown in Fig. 4. The carbon atoms although not needed by NanoCap are produced by default. For each point P at position (px , pz ), the position of the A and B carbon atoms are given by:

chiral vector shown is for the (4,2) nanotube.

˚. where ac is the carbon bond length of 1.421 A The properties, symmetry and caps of a nanotube depend on the orientation of the underlying graphene sheet. To describe this orientation, a vector is introduced, namely the chiral vector C which is defined in terms of a1 and a2 : C = (n, m) = na1 + ma2

(4)

The magnitude of C gives the circumference of the nanotube and as such the cylindrical radius rt is given by:

A = (px , pz ) B = (px + ac , pz )

|C| (5) 2π which is used to determine the scaling factor γ to reduce the nanotube to a cylinder of unit radius. (γ=1/rt ). The angle C subtends with the axis of the graphene sheet is labelled the chiral angle θC as shown in Fig. 3. Two special cases of nanotube are constructed when θC equals 0◦ [C=(n, 0)] and 30◦ [C=(n, n)]. These achiral nanotubes are known as the zigzag and armchair respectively and have additional mirror plane symmetry when compared to chiral [C=(n, m)] nanotubes. Perpendicular to C is the vector T that defines the axial direction of the nanotube: rt =

T = (−Cz , Cx )

(10)

The dual lattice point D which is fundamental to the operation of NanoCap is simply offset along the x direction to the centre of a hexagon: D = (px + 2ac , pz )

(11)

The final three points labelled I1−3 represent a po0 tential C2 axis of rotational symmetry once the 3D nanotube is constructed. The position of these points on the 2D lattice are given by: I1 = (px + ac /2, pz ) I2 = (px + 5ac /4, pz + I3 = (px + 5ac /4, pz −

(6)

b and T b form a new orthonormal coorThe vectors C dinate system that can be used to align the nanotube

(9)

√

√

(12) 3ac /4)

(13)

3ac /4)

(14)

These points are used to align the 2D lattice such that once in 3D, there exists a simple 180◦ rotation to map one end of the nanotube to the other. This 4

jected onto C is proportional to the angle around the

work of Saito et al. Using the 2 atom basis of the T.that All atom positions are generated from i=0 which is used to wrap positions of A atoms leave The radius of unit the cell. nanotube rt distance along graphene lattice, thenanotube. position of the i-th cylindrical A atom is the nanotube The additional where NH is the number of hexagons in the gra defined simply as iR.isThe B atom is thenby o↵set also defined C:from T to the centre of a hexagon is given by: sheet: this position along a proportion of Ch and T. All h⇡ i atom positions are generated from i=0 to Nhex , where |C| ✓Ch B = ac · sin Nhex is the number of hexagons in the graphene sheet. 6 (5) rt = (13) NH = 2(n2 + m2 + nm)/dR 2⇡ Application of the symmetry vector R to all sites unhex = 2 B

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

2 which is used to determine the scaling factor to When the application of the symmetry vecto 5. CapofDual Lattice Initialisation reduce the nanotube to a cylinder unit radius. erates coordinates outside of the nanotube cel ( =1/rt ). tions are wrapped using the appropriate pro The angle C subtends with theUpon axis ofconstruction the graphene of the nanotube of the required T onto C and T. number sheet ° is labelled the chiral chirality, angle ✓C the as shown in of dual lattice points in the tube As introduced previously, the algorithm f 0 Fig 3. Two special cases of nanotube are usedare toconstructed estimate the construction number of points thatupon should is based solving the Th when ✓C equals 0 [C=(n, 0)] and 30 [C=(n, n)]. be used in the generationproblem of the caps. estimate using This the dual latticeis presentation These achiral nanotubes are known as the zigzag and extrapolated from the density of dual lattice points in graphene network. Therefore, the two atom b C I2 armchair respectively and have additional mirror modified to incorporate a dual lattice point, the nanotube. It should be noted that for nanotubes 30° plane symmetry when compared to chiral [C=(n, m)] is positioned in the centre of a hexagon as sh A I1 B D that have a small radius, this estimate will be lower I3 nanotubes. Fig 4. Upon construction of the nanotube, thi a1 than T the ideal number points. For all cases of cap Perpendicular to C is the vector that defines the of tube ND =NH dual lattice points. In addition to th axial length of the nanotube construction unit cell. Although not it is recommended to sample a range of z eration of carbon atoms and dual lattice points necessary for cap construction, T is defined such that dual lattice points, either sidebasis of the estimated num- These poin other points are constructed. a2 x the nanotube is periodic alongber. the nanotube axis. As resent intersections of local carbon bonds (wh such, T extends to the atom corresponding to the Generation of the initial points is carried ofout also cap located at intersections neighbouring du firstand atom at the origin of 2D unit cell and is given in Figure 4: Basis positions of the atoms points associated tice points) and for are the denoted I1 to I3 . Each o in a similar manner to that described initialof a1 and : with the 2D nanotube sheet. A andterms B represent thea2carbon pointslattice. represents a potential C2 axis of rot isation of the fullerene dual The points are atoms, D indicates the position of the dual lattice point and symmetry once the 3D nanotube is constructed along the = t1 a1 +produced t2 a2 (6)negative z coordinate, attaching I1−3 give the three intersections of carbon-carbon bondsTwhich is useful in later routines involving transform 0 to the nanotube at z=0. This is achieved by modrepresent C2 rotational axis of symmetry once the 3D tube As T defines the smallest periodic unit, the coeffiof the final cap structure. The full basis is is constructed. Repeating this basis for each 2D lattice point ifyingdivisors equation 1 for such that These dual cients t and t2 have no common except in Figz40 =[−1,0]. and by translation using R produces generates all atoms and points required for 1the nanotube cap lattice points belonging points to therequired cap are free to move unity and are given by: for nanotube construction. construction.

during the minimisation 4 process. Currently, a single cap is constructed at one end of the nanotube which is then rotated 180◦ about the x axis to cap the alternate end. This is possi0 ble due to the alignment of the C2 axis with the x axis during the construction of the nanotube. Producing identical caps at either end of the nanotube is important when determining cap energies as in our previous work [14]. As an alternative, different caps could be produced by repeating the initialisation, optimisation and triangulation processes for each end of the nanotube. Currently, the NanoCap software is constrained to produce identical cap structures.

is achieved by determining the point which intersects with the perpendicular bisector to T. This point is used to shift the 2D lattice such that 3D x axis of the 0 nanotube is inline with the C2 axis of rotation. Once constructed the 2D lattice is reorientated b and T b align with the x and z cartesian such that C axis. The dual lattice points are then shifted in the z direction such that the boundary is at z=0. The transformation of the 2D lattice points into the 3D nanotube is straightforward. As the z position remains the same in 3D as in 2D, the only coordinate to consider is along the x axis. The position of each point i along the 2D x-axis gives the angle around the circumference of the nanotube: θi = 2π

x2D i |C|

6. Dual Lattice Optimisation As introduced previously, optimising the dual lattice corresponds to finding a solution to the Thomson problem. For a given set of ND points, this involves minimising the total potential energy:

(15)

This angle is used to determine the cartesian coordinates of each point in the 3D xy plane: xi = rt cos(θi ) yi = rt sin(θi )

φ=

ND X ND X

i=1 j=i+1

(16)

1 |ri − rj |

(17)

which is analogous to the total electrostatic energy of a system of point charges. The algorithm outlined in the present work centres around minimising this potential energy for the dual lattice points constructed for either the fullerene or capped nanotube topologies. The process of minimisation of the fullerene

Once created, the dual lattice is scaled to a unit cylinder using γ defined previously. The dual lattice points belonging to the nanotube are held fixed during the minimisation process. 5

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

for the fullerene construction. To determine the tube points involved in the energy minimisation, a cutoff Zc is introduced along the tube axis which depends on the number of cap points Ncap D :

dual lattice points is directly in line with traditional approaches to solving the Thomson problem. At each iteration of the minimisation algorithm, the points are normalised back to the surface of the sphere. In addition, the radial component of force is removed from each atom, ensuring all forces act tangentially to the sphere’s surface. The algorithm adopted for the minimisation of the dual lattice is an implementation of the limited-memory Broyden-Fletcher-Goldfarb-Shanno (L-BFGS) method [17, 18, 19] as included in the SciPy optimisation libraries [21]. The method circumvents direct calculation of the Hessian matrix by continual updates and corrections during optimisation.

Ncap Zc (ρ) = A exp (µρ ) , ρ = D 2π α

(18)

where A= 0.790378, µ = 1.62583 and α= 0.251753. Although this cutoff is calculated automatically by default, it can be manually overridden in situations where the cap density is significantly greater than the tube density. 7. Escaping Minima As discussed in the literature regarding finding solutions to the Thomson problem, as the number of points increases the number of local minima grows exponentially [22]. For this reason, the code includes a tool for minima searching. This involves looping through the procedures for dual lattice minimisation, triangulation and if selected, the minimisation of the resulting carbon lattice using a physical carbon potential. The user defines the extent of the search by inputting the number of required unique minima and the maximum number of minima to search. After each successful minimisation, there are several options to escape the local potential energy basin. The two simplest methods are to either randomly offset the dual lattice points from the minima or to reset them completely. Resetting the structures can be very effective for systems with a large number of well separated local minima and can be quick to produce a multitude of structures. Randomly offsetting the dual lattice points is also effective and the minimisation process is typically quicker than a complete reset due to the closer proximity to a minimum. Importantly the perturbation is constrained to be tangential to the surface of either the sphere or cylinder. Also, in the case of nanotube cap generation, care is taken as to ensure no cap points are offset into the tube as points may become too close to the fixed points belonging to the tube. This ensures sensible initial forces during optimisation. The magnitude of the random tangential perturbation is determined by the nearest neighbour separation of the current set of points. Although fast, resetting or offsetting the system in the hope to find a new basin is not reliable and can result in revisiting the same minima, particularly if

6.1. Modifications for Capping Nanotubes In contrast to the fullerene dual lattice minimisation which is a direct analogue to solving the Thomson problem, the optimisation procedure associated with the capped nanotube dual lattice requires important modifications. Firstly, only the cap dual lattice points are free to move during minimisation, with the points generated on the tube held fixed. The implementation of this is trivial and involves the multiplication of the force by a binary mask of length 3ND , which contains zeros for the fixed points. A further adaption of the minimisation process specific to capping nanotubes is the surface to which the points are normalised. Dependent on which side of the tube-cap boundary a point lies, it is either scaled to the unit hemisphere or cylinder. This is an important feature as it allows cap points to move into the nanotube region, which is a necessity for highly chiral tubes where the tube boundary may be coarse. A final and vital modification specific to capping nanotubes is associated with the range of the potential energy function. The introduction of the tube points which are held fixed generates a significant net repulsion towards the cap points. For long nanotubes, this can cause clustering of the cap points at the apex of cap. There are two solutions to this problem; truncate the potential at a given pair separation or restrict the number of tube points included in the force evaluation. Using the first option, cap points were found to penetrate the tube resulting in the need for different truncation criteria for the cap and tube points. The second option was found to be much more reliable and involved fewer modifications to the generalised optimisation routines implemented 6

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

potential energy surface may be modified to such an extent that the structure search fails completely. Gaussian functions were chosen due the simple form of the derivatives with respect a component of the position vector rα : d −RT dφg (R∆ ) ∆ AR∆ = φg (R∆ ) · (22) drα drα

the system is in a wide basin. Therefore as a final option, the system with position vector R can escape the current minimum by iteratively climbing out of the basin following the gradient of the potential or the negative direction of force F: Ri+1 = Ri − αFi

(19)

where i denotes the iteration number and α is a variable step size dependent on the change in the magnitude of force per iteration. When the system leaves the vicinity of the current basin, the projection of force onto the separation vector changes sign: (Ri+1 − Ri ) · Fi

which allows for fast force evaluation. 8. Triangulation Upon successful termination of the minimisation process, the dual lattice points represent a minimum energy structure with regards to the potential in Eq. 17. To construct the carbon lattice, the face dual of the dual lattice network is generated. This is achieved by reversing the dual lattice transformation shown in Figure 1 which requires triangulation of the dual lattice points. There is a significant literature and knowledge base regarding triangulation algorithms. Many of these algorithms concern much more complex topologies where the neighbourhood of each point varies greatly. For this reason, a simple procedure is adopted based upon 3D Delauny triangulation. This involves constructing triangles such that no point lies within the circumcircle created by each triangles vertices. As the routine progresses, the normals of each triangle are stored and are used in a secondary algorithm which ensures no triangles are constructed inside the closed surface. This is accomplished by checking the intersections of the forward and backward facing normals with other triangles. Any normal that intersects multiple triangles is flagged and the corresponding triangle is removed. This is an important check for nanotubes which have a diameter that is of a similar magnitude as the dual lattice point separation, for example the (5,0) nanotube. Due to the various definitions of the centre of a triangle, the carbon lattice may be constructed in a number of different ways. Currently NanoCap places a carbon atom at the centroid of each triangle as this has been found to give the best spacing between atoms. This choice is only significant for the fullerene and cap regions as the dual lattice points belonging to the nanotube produce an equilateral triangulated mesh, for which each centre is coincident. The triangulation routine is the first generalised module, working on fullerene and capped nanotube

(20)

This ensures the system visits a new basin, although does not guarantee the resultant structure will be symmetrically unique. As the algorithm only requires a method of escaping a minimum, advanced saddle point finding methods are not required. Currently, structures are determined to be unique by comparison of the total dual lattice energy. Future revisions will introduce the detection of symmetry equivalent structures. To encourage the sampling of different minima during the structure search, an option to add 3ND dimensional Gaussians to the potential energy function has been implemented. If enabled, after each dual lattice optimisation stage a Gaussian is placed at the location of the new minima. In future steps of the structure search the total potential energy used during the dual lattice optimisation then has an additional contribution from previously placed Gaussians. This additional potential for each Gaussian g takes the form: φg (R∆ ) = H exp −RT ∆ AR∆ (21) R∆ = R − Rg where R and Rg are the 3ND position vectors of the the dual lattice points and the Gaussian respectively. The matrix A contains 1/2σ 2 on the diagonal. The height H and width σ of the Gaussian are user defined parameters and should ideally be significantly smaller than the widths and heights of potential wells on the dual lattice energy surface. Typical parameters used during development of NanoCap range from 0.1 to 0.5 for systems containing up to a few hundred dual lattice points. If these parameters are too small the structure search will take a long time to locate a new minima, yet clearly if they are too large then the 7

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

a sensible scale, the structure is fully optimised using the same L-BFGS algorithm described previously [17, 18, 19, 21]. Both the scaled and fully optimised structures are stored and the associated atomic coordinates can be output to file. The scaled structures are useful for the construction of concentric carbon fullerenes (carbon onions) or capped multiwalled carbon nanotubes, as they allow for a uniform interlayer separation within the spherical regions. (a)

(b)

10. Output and Analysis At any time during a NanoCap session, structures can be saved to disk. The dual lattice, constrained carbon lattice and fully optimised carbon lattice can be saved in the common .xyz file format along with information relating to the structure, such as the ring statistics. In addition, if the GUI version of NanoCap is used, the Schlegel diagram can be saved as an image along with a isometric view of the structure. Outputted images can be encoded with software such as FFMpeg to produce animations of the structure.

Figure 5: Minimised dual lattice of the capped (23,17) nanotube with 444 carbon atoms in the cap. (a) Triangulation of the dual lattice is shown in grey with the cap dual lattice points shown in white. (b) Rendering of carbon rings with pentagons in blue, hexagons in green and heptagons in red.

dual lattice points alike. After triangulation, a single set of carbon atoms are produced which are used in later analysis and minimisation routines. 9. Carbon Lattice Minimisation

10.1. Ring Counting

As the fullerenes and capped nanotubes constructed from the dual lattice only represent sensible 3-fold topologies, an accurate physical model of carbon is required to produce the final atomic coordinates. Currently, the Environmental Dependent Interatomic Potential (EDIP) [23] is implemented within the code. EDIP provides a suitably physical model of carbon without the computational expensive of first principles methods. Future releases of NanoCap will incorporate other empirical carbon potentials, in particular those accessible through The Large-scale Atomic/Molecular Massively Parallel Simulator (LAMMPS) [24] using the already developed Python interface. The carbon potential is used in a two stage process to produce the fully relaxed carbon structures. Firstly, the structures are scaled from the unit radius topologies outputted from the dual lattice minimisation procedure. For fullerenes, an initial estimate of the scale factor is determined using the known C60 radius. For capped nanotubes, an estimate is already known as the radius of the uncapped nanotube has been defined (Eq. 5). To determine the precise scale factor, constrained optimisation is performed using the Nelder-Mead simplex algorithm [25] as implemented in the SciPy libraries [21]. Once at

Ring counting is carried out using the approach outlined by Franzblau [26]. The method is centred around identifying all shortest path (SP) rings in a network where the connectivity is known. For each atom i in the constructed fullerene or capped nanotube, a neighbour list is generated and all rings involving atom i are identified. For each ring, a distance is computed between each vertex in terms of the number of intermediate vertices. If these distances do not correspond to the true distances in the full network, then the ring is not an SP ring and is discarded. Importantly, after all SP rings have been determined for atom i, it is removed from the full network of atoms. This removes all rings associated with atom i and eliminate the possibility for double counting. The application of this method is made possible using recursive algorithms, for both the generation of all rings containing vertex i and for the determination of SP rings. 10.2. Schlegel Transformation In additional to the 3D rendering of the final structures NanoCap also includes the option to render the 2D Schlegel diagram. This represents the projection of the 3D network onto a plane and is particularly useful for the examination of the topology of capped 8

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

nanotubes. By default projection is carried out into the xy plane, inline with the nanotube orientation along the z axis. The projected 2D position r0i of each atom or point i is then given by: ri = (xi , yi , 0) r0i = ri + γs ˆri

11. Implementation and Source Code The NanoCap framework is implemented in Python, with computationally expensive algorithms written in C and compiled as shared libraries. NanoCap is designed to be used as both a standalone application complete with a GUI and with 3D rendering capabilities and also as libraries to be used in Python scripts. To achieve this, the code takes advantage of the versatile object orientated nature of Python with core classes and routines separated from GUI and rendering elements. In addition, as Python is an interpreted language with relatively simple syntax, users with little programming experience can quickly produce custom scripts that access the complete functionality of the NanoCap libraries.

(23)

where γs controls the extent of the projection in the plane with a value of γs =0 resulting in a direct projection. A cutoff along the z axis, rs is also incorporated which determines which points or atoms are used in the Schlegel construction. This is useful when only the capped region of a nanotube is required. Examples of a Schlegel diagrams for a range of capped nanotubes are shown in Fig 6.

11.1. Core classes The core classes and routines in NanoCap (nanocap.core, nanocap.structures, nanocap.ext) contain the main functionality for fullerene or capped nanotube construction. These modules can be used as libraries in Python scripts to produce structures quickly or in bulk. Only the NumPy [20] and SciPy [21] packages are required when using NanoCap as a library. An example script that uses the libraries to produce capped (10,10) nanotubes can be found in Figure 7. This script could readily be modified to run in parallel either locally on multiple threads or distributed to separate cpu nodes using MPI (or a Python wrapper such as MPI4Py [27]).

(a) (7,7)

(b) (10,3)

11.2. GUI and rendering The NanoCap graphic user interface (GUI) is implemented using the Qt framework [28], using PySide bindings. Rendering is carried out using the Visualisation Toolkit (VTK) [29] which again is accessed through Python wrappers. The main advantage of using the GUI enabled version of NanoCap is the ability to visual inspect each new structure during generation. As a new structure is found, the user is presented with a 3D visualisation which can be interactive manipulated whilst the structure search continues. Each structure is dynamically entered into a structure table, which the user can view and use to load previously found structures.

(c) (23,17) Figure 6: Fully optimised 3D isometric and 2D Schlegel views of a range of capped nanotubes. (a) The (7,7) nanotube with a 44 atom cap. (b) A capped (10,3) nanotube containing 50 carbon atoms. (c) The (23,17) nanotube with a cap containing 444 carbon atoms which includes heptagon ring structures.

9

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

12. Summary NanoCap is a simple and generic application for the construction of low energy fullerene and capped nanotube structures. It provides an ideal tool to accompany the study of finite carbon molecules using atomistic computer simulation. The implementation involves a standalone application which includes a GUI and allows for dynamic visual inspection through 3D rendering. In addition, the NanoCap libraries can be used in custom Python scripts that enabled the user to produce structures in bulk or to include the structure generation routines into pre-existing code. 13. References References [1] G. Brinkmann and A. W. Dress, J. Algorithms 23, 345 (1997). [2] G. Brinkmann, U. Nathusius, and A. Palser, Discret. Appl. Math. 116, 55 (2002). [3] Nanotube Modeler - http://www.jcrystal.com/ [4] Atomistix ToolKit - http://www.quantumwise.com/ [5] D. J. Wales, H. McKay, and E. L. Altschuler, Phys. Rev. B 79, 224115 (2009). [6] D. J. Wales and S. Ulker, Phys. Rev. B 74, 212101 (2006). [7] E. L. Altschuler and A. P´erez-Garrido, Phys. Rev. E 71, 1 (2005). [8] A. P´erez-Garrido, Phys. Rev. B 62, 6979 (2000). [9] E. L. Altschuler and A. P´erez-Garrido, Phys. Rev. E 73, 36108 (2006). [10] A. P´erez-Garrido and M. A. Moore, Phys. Rev. B 60, 15628 (1999). [11] A. P´erez-Garrido, M. Ortu˜ no, E. Cuevas, and J. Ruiz, J. Phys. A. Math. Gen. 29, 1973 (1996). [12] J. R. Edmundson, Acta Crystallogr. Sect. A Found. Crystallogr. 48, 60 (1992). [13] J. R. Edmundson, Acta Crystallogr. Sect. A Found. Crystallogr. 49, 648 (1993). [14] M. Robinson, I. Suarez-Martinez, and N. A. Marks, Phys. Rev. B 87, 155430 (2013). [15] R. Saito, G. Dresselhaus, and M. S. Dresselhaus, Physical Properties of Carbon Nanotubes (1998). [16] E. B. Barros, A. Jorio, G. G. Samsonidze, R. B. Capaz, A. G. Souza Filho, J. Mendes Filho, G. Dresselhaus, and M. S. Dresselhaus, Phys. Rep. 431, 261 (2006). [17] C. Zhu, R. H. Byrd, P. Lu, and J. Nocedal, ACM Trans. Math. Softw. 23, 550 (1997). [18] R. Byrd, P. Lu, J. Nocedal, and C. Zhu, SIAM J. Sci. Comput. 16, 1190 (1995). [19] J. L. Morales and J. Nocedal, ACM Trans. Math. Softw. 38, 1 (2011). [20] T. E. Oliphant. Comp. Sci. Eng. 9(3):1020 (2007). http://www.numpy.org [21] E. Jones, T. E. Oliphant, and P. Peterson, SciPy: Open Source Scientific Tools for Python http://www.scipy.org/.

Figure 7: Example Python script that uses the NanoCap libraries to create and save 5 capped (10,10) nanotubes of around 10 ˚ A in length.

11.3. External libraries Currently, the only external library included in NanoCap is EDIP. Other libraries such as the LAMMPS Python [24] module will be implemented in future releases. The Fortran source code for EDIP is compiled as a shared object and imported into Python using the ctypes library. To access the internal force and position arrays in EDIP, additional Fortran modules were written to serve as an interface. These access points are used by a Python interface that contains routines for EDIP initialisation, passing atomic coordinates and retrieving forces and energies. All external libraries are stored in the ext directory of the source. 10

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65

[22] T. Erber and G. M. Hockney, Phys. Rev. Lett. 74, 1482 (1995). [23] N. A. Marks, Phys. Rev. B 63, 035401 (2000). [24] S. Plimpton, J. Comput. Phys. 117, 1 (1995). [25] J. A. Nelder and R. Mead, Comput. J. 7, 308 (1965). [26] D. Franzblau, Phys. Rev. B 44, 4925 (1991). [27] MPI4Py - MPI for Python. http://mpi4py.scipy.org/ [28] Digia, Qt - Cross-platform application and UI framework http://www.qt-project.org/. [29] W. Schroeder, K. Martin, and B. Lorensen, The Visualisation Toolkit (VTK) - Copyright (c) 1993-2008 http://www.vtk.org/.

11

Copyright © 2024 C.COEK.INFO. All rights reserved.